CHAPTER 1: OVERVIEW AND PHYSICAL KEY CONCEPTS
1.3. Radiation damage and radiation effects in A15 superconductors
1.3.3. Radiation effects in superconductors
A large number of publications on the effects of radiation damage in superconductors has been published since 1970, the projectiles being protons, neutrons and heavy ions. All these irradiation types were found to induce a certain amount of disorder in the A15 phase, depending on the projectile. As a result the critical properties (Tc, Jc and Bc2) change, the lattice parameter increases, the electronic specific heat decreases and the electrical resistivity is enhanced. A flowchart of the effects of high energy radiation on A15 type compounds is reported in Figure 18 .
Aronin  proposed an exponential function to describe the decrease of the Bragg Williams long range order parameter S with increasing fast neutron fluence, 𝜙𝜙𝑑𝑑:
𝑆𝑆(𝜙𝜙𝑑𝑑) =𝑆𝑆(0)𝑒𝑒−𝑘𝑘𝑘𝑘𝑡𝑡 27
In equation 27, the factor 𝑆𝑆(0) is the 𝑆𝑆 value before irradiation, and 𝑏𝑏 is a constant which depends on the material. Since increasing particle fluence causes a decrease of 𝑆𝑆, the mean free path 𝑙𝑙 of the electrons will decrease (see also Subsection 1.2.3).
In the following an overview of the main changes induced by high energy proton and neutron irradiation on the intrinsic properties of A15 superconductors, especially for Nb3Sn, will be given and the physical reason behind these changes will be discussed.
Figure 18 Schematic representation of the radiation induced effects in A15 type compounds, with increasing fluence. Extracted from Ref. .
Changes in Tc after irradiation
In 1974 Bett  reported a gradual decrease of 𝑇𝑇𝑐𝑐 in Nb3Sn up to a fast neutron fluence of about 2×1023 n/m2. Weiss et al.  found that the variation of 𝑇𝑇𝑐𝑐 at low fluences is linear for both binary and alloyed wires: the 𝑇𝑇𝑐𝑐 reduction is close to 4% for 14MeV neutron fluences up to 1022 n/m2 and reaches about 20% for higher fluences. At the highest fluences, i.e. 4×1022 n/m2, they found that the variation Δ𝑇𝑇 for alloyed wires (- 2.9 K for Ti additions and -3.3 K for Ta additions) was slightly higher than for binary wires varies (from -2.3 to -2.6 K). As shown recently by Flükiger et al. , the fact that Ta and Ti occupy different lattice sites before
irradiation (Ta on Nb sites, Ti on Sn sites) may give an explanation for the observed difference in the decrease of 𝑇𝑇𝑐𝑐 for the two types of alloyed Nb3Sn wires. The decrease of 𝑇𝑇𝑐𝑐 in multifilamentary Nb3Sn wires was also observed by Hahn , who found for 14.8 MeV neutron irradiation an exponential fit of the form:
𝑇𝑇𝑐𝑐(𝜙𝜙𝑑𝑑) =𝑇𝑇𝑐𝑐0𝑒𝑒−𝑘𝑘𝑘𝑘𝑡𝑡 28 where 𝑇𝑇𝑐𝑐0 is the critical temperature before irradiation and 𝑏𝑏 is a fit parameter with values between 0.062 and 0.082 for binary wires and between 0.081 and 0.098 for alloyed wires up to a fluence of ~ 1022 n/m2. Due to the small value of 𝑏𝑏 the exponential dependence of 𝑇𝑇𝑐𝑐 with fluence given in equation 28 is almost linear at not too high fluences, in agreement with the results found by Bett et al.  and Weiss et al. .
The debate on the defect mechanisms responsible for the decrease of 𝑇𝑇𝑐𝑐 is very complex and the question on how the radiation damage affects the critical temperature remains still open. Four main candidates are used in literature to explain the degradation of 𝑇𝑇𝑐𝑐 with fluence, i.e.:
1) Decrease of the atomic order parameter S due to site exchanges (“antisite defects”) The Bragg Williams LRO parameter, 𝑆𝑆, defined in Subsection 1.2.2 is a function of the occupation number and of Sn composition. Appel  provided a detailed theory on a uniform distribution of site exchanges in irradiated compounds based on McMillan theory  (strong coupling theory), the electron-phonon interaction parameter λ(S) in his theory being a function of the long-range order parameter. A decrease of 𝑆𝑆 in irradiated A15 compounds was observed in Nb3Al by Sweedler et al. , in Nb3Pt by Moehlecke et al.  and in V3Si by Cox and Tarvin . A homogeneous distribution of the damage in A15 type compounds was also proven on the basis of low temperature specific heat measurements before and after irradiation. Viswanathan et al. [76, 77] and Cort et al.  found that the superconducting transition widths of the A15 type compounds V3Si and Nb3Al remain narrow after neutron irradiation (≥1 MeV). In particular for Nb3Al, the width of the specific heat jump, ∆𝑇𝑇𝑐𝑐, increases from 0.8 K in the unirradiated state to 1.3 K after 1.3×1023 n/m2, where the 𝑇𝑇𝑐𝑐/𝑇𝑇𝑐𝑐0 is equal to 0.51; for V3Si, an increase of ∆Tc from 0.5 to 1.2 K was observed after 2.22×1023 n/m2, where 𝑇𝑇𝑐𝑐/𝑇𝑇𝑐𝑐0= 0.4. In both cases there is thus still a high degree of homogeneity in the LRO
parameter S. This is analogous to the case of fast quenching of A15 type compounds, where the total gradient across the sample is only 𝛿𝛿𝑆𝑆 ≤0.02, as shown by Flükiger .
From X - ray diffractometry, Sweedler et al.  found an exponential dependence of the critical temperature of Nb3Sn on 𝑆𝑆:
𝑇𝑇𝑐𝑐(𝜙𝜙𝑑𝑑) =𝑇𝑇𝑐𝑐0𝑒𝑒−𝐶𝐶(1−𝑆𝑆/𝑆𝑆(0)) 29 assuming an initial value for long range order parameter 𝑆𝑆(0) = 1 (the experimental proof for perfect ordering in Nb3Sn is given in the present work, see Section 4.2), they found a value of 5.0±1.5 for the constant C and concluded that the decrease of Tc at doses up to 1023 n/m2 (where Tc/Tc0 ~ 0.5) is mainly caused by a decrease of the long-range atomic order parameter, 𝑆𝑆 [79, 80].
2) The formation of depleted zones (inhomogeneous disorder)
By means of TEM analysis of neutron irradiated Nb3Sn bronze wires, Pande 
observed in 1977 small “disordered micro-region” of about 4 nm size, embedded in a much less disordered matrix. Since the critical temperature of these disordered regions was significantly lower than that of the matrix Pande  concluded that the critical temperature of the system would be strongly depressed due to the proximity effect.
Consequently he suggested an inhomogeneous disorder after irradiation. However calorimetric measurements [76, 77] constitute a definitive proof for the validity of the homogeneous disordering model proposed by Sweedler et al. [82, 80]. This will be discussed in detail in the following.
3) The increase of the mean static displacements of atoms, 𝑢𝑢
Meyer et al.  and Testardi et al.  observed an increase of the mean static displacements of atoms after heavy irradiation of V3Si single crystals by means of the channeling technique. Earlier to these observations, a weakening of the X – ray line intensities at high 2θ angles had been observed by Testardi et al.  and Poate et al.
 on irradiated Nb3Ge and Nb3Sn. This weakening could neither be accounted for by a lowering of the LRO parameter nor by a particular choice of the temperature factor: it was found to be related to static displacements of the chain atoms from their ideal lattice
sites. Later on, the same authors determined the quantity 𝑢𝑢 by means of X – ray diffraction measurements [87, 88]. After their first detection, the static displacements were invoked as being the main responsible for the initial decrease of 𝑇𝑇𝑐𝑐 after high energy irradiation [84, 89]. Schneider et al.  found, however, that after proton irradiations the displacements were substantially different from zero after higher doses only. After Schneider  various studies were performed to clarify the correlation between the decrease of 𝑇𝑇𝑐𝑐 and the increase of 𝑢𝑢 [80, 83, 84, 90]. However since the same value of 𝑇𝑇𝑐𝑐 correspond to very different values of 𝑢𝑢, this indicates that static displacements, which occur simultaneously to atomic site exchanges, are not the dominant factor causing the initial decrease of 𝑇𝑇𝑐𝑐 in high 𝑇𝑇𝑐𝑐 A15 type compounds .
4) The mechanical effects (stress - strain effects)
Radiation hardening of the Cu matrix after irradiation induce a pre-stress on Nb3Sn matrix, and can thus lead to a reduction of 𝑇𝑇𝑐𝑐. Okada et al.  have experimentally found that after neutron irradiation up to 3.6×1023 n/m2 the enhancement of the pre-strain ε is about 0.2 %. However, the fluences corresponding to the maximum of 𝐽𝐽𝑐𝑐 after neutron irradiation are about one order of magnitude smaller, which would lead to an enhancement Δ𝜀𝜀 of 0.02 % only. It follows that up to these fluences the effect on the pre-strain is almost negligible. This is confirmed by the first principles calculations by De Marzi and coworkers , who found that, the variation of 𝑇𝑇𝑐𝑐 is very small: about 0.05 K. Thus at low fluences, i.e. up to values corresponding to Jc/Jcmax, the additional effect of the radiation induced pre-strain on 𝑇𝑇𝑐𝑐 can be neglected.
As will be explained in the following, the homogeneous decrease of S is the main responsible for the observed decrease of 𝑇𝑇𝑐𝑐 up to radiation doses of ~ 1023 n/m2, while inhomogeneous defects, mean static displacement and mechanical effects are dominant for higher doses only, where the value of 𝑇𝑇𝑐𝑐 is too low for being of interest for the present work.
Two main arguments can be invoked for proving the validity of antisite defects as the dominant mechanism :
a. Homogeneous distribution of antisite defects after irradiation detected by specific heat measurements.
The question about a homogeneous distribution of the damage can be answered on the basis of the known low temperature specific heat measurements before and after irradiation for the A15 type compounds Nb3Sn by Karkin et al. , Nb3Al by Cort et al.
 and V3Si by Viswanathan et al. . For the three systems, heavy neutron irradiations up to fluences of 2×1023 n/m2 causes a very small enhancement of the transition width, Δ𝑇𝑇𝑐𝑐, i.e. for a neutron fluence reducing 𝑇𝑇𝑐𝑐 to about 50% of the initial value, the transition width Δ𝑇𝑇𝑐𝑐 is only enhanced by ≤ 1K. In addition in the specific heat curves, there is no trace of the original superconducting transition temperature, 𝑇𝑇𝑐𝑐0, in any of the three systems after irradiation. This implies that the amount of depleted zones (with considerably lower 𝑇𝑇𝑐𝑐) is very small and cannot account for the observed decrease of the superstructure lines, i.e. indirectly that the damage is homogeneous up to 1023 n/m2.
b. Comparison between the variation of 𝑇𝑇𝑐𝑐 vs. the order parameter S after irradiation and after fast quenching by diffraction methods.
No direct comparison between neutron irradiation and quenching has been performed on Nb3Sn and the data reported here concern the system Nb3Pt, another A15 type compound. Figure 19 shows the variation of 𝑇𝑇𝑐𝑐 for Nb3Pt vs. the long range order parameter, S, after fast quenching from temperatures up to 1900 °C by Flükiger et al.
 and after neutron irradiation (E>1 MeV) by Moehlecke et al. . It follows from Figure 19 that the variation of 𝑇𝑇𝑐𝑐 vs 𝑆𝑆 is the same, regardless whether the compound was fast quenched or irradiated. Since quench induced disordering constitutes a particularly simple case, where the only possible defects are the antisite defects (up to a few %) and quenched-in vacancies (≤ 0.02 % at 300 K), the same behavior found after quenching and after irradiation constitutes an additional argument in favor of the antisite defects mechanism for the observed decrease of 𝑇𝑇𝑐𝑐 after irradiation up to fluences of 1023 n/m2.
Changes in Bc2 and Jc after irradiation
Weiss et al.  found that after high energy irradiation the upper critical field increases up to 1022 n/m2 and then decreases at higher fluences. The reason for the increase of 𝐵𝐵𝑐𝑐2 with fluence can be explained by the increase of the residual electrical resistivity, 𝜌𝜌0. Indeed, Alterovitz et al.
 observed that after irradiation of V3Si bulk sample by 35 MeV protons at fluences up to 1021 p/m2 the enhancement of 𝜌𝜌0 (due to the decrease of the electronic mean free path) prevails on the decrease of 𝑇𝑇𝑐𝑐, thus the increase of 𝐵𝐵𝑐𝑐2 follows the trend of 𝜌𝜌0. At higher fluences the tendency of 𝜌𝜌0 and 𝑇𝑇𝑐𝑐 with fluence is reversed and it is suggested that the decrease of Bc2 at fluences beyond those corresponding to the maximum of 𝐽𝐽𝑐𝑐/𝐽𝐽𝑐𝑐0 is mainly due to the degradation of 𝑇𝑇𝑐𝑐.
Figure 19 Tc vs. long-range order parameter S (determined by X ray diffraction) for Nb3Pt after fast quenching from different temperatures (Flükiger et al. ) and after neutron irradiation (Moehlecke et al.
An analogous behavior of the critical current density with fluence was found by many authors and the existence of the maximum in 𝐽𝐽𝑐𝑐 at which the maximum of 𝐵𝐵𝑐𝑐2 occurs at almost the same fluence suggests that the enhancement in 𝐽𝐽𝑐𝑐 was correlated to that one of 𝐵𝐵𝑐𝑐2 [98, 73]. Later on, however, it has been shown by Küpfer et al.  that after high energy irradiation the change in 𝐵𝐵𝑐𝑐2 is not the main reason for the enhancement of 𝐽𝐽𝑐𝑐, at least at low fluences when both these parameters increase. Indeed, these authors found that the enhancement of 𝐽𝐽𝑐𝑐 after neutron